Poisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics


 Dora Hicks
 1 years ago
 Views:
Transcription
1 /j x Poisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics W. VAN PAEPEGEM, I. DE BAERE, E. LAMKANFI and J. DEGRIECK Ghent University, Department of Mechanical Construction and Production, SintPietersnieuwstraat 41, 9000 Gent, Belgium Received in final form 10 October 2006 ABSTRACT Even if the extent of damage in fibrereinforced plastics is limited, it already affects the elastic properties. Therefore, the damage initiation and propagation in composite structures is monitored very carefully. Beside the use of nondestructive testing methods (ultrasonic inspection, optical fibre sensing), the followup of the degradation of engineering properties such as the stiffness is a common approach. In this paper, it is investigated if the Poisson s ratio can be used as a sensitive indicator of (fatigue) damage in fibrereinforced plastics. Static, cyclic and fatigue tests have been performed on [0 /90 ] 2s glass/epoxy laminates, and axial and transverse strain were measured continuously. The evolution of the Poisson s ratio versus time and axial strain is studied. It is concluded that the degradation of the Poisson s ratio can be a valuable indicator of damage, in combination with the stiffness degradation. Keywords damage mechanics;fatigue;finite element analysis;polymermatrix composites (PMCs). INTRODUCTION Damage in fibrereinforced composites can take many forms: 1,2 (i) matrix cracks, (ii) fibrematrix interface failure, (iii) fibre pullout, (iv) delaminations and (v) fibre fracture. This damage affects the value of the elastic properties at an early stage. Especially in fatigue, the damage initiation phase can cause a pronounced drop of the elastic modulus of 5 10%. In the next damage propagation phase, the stiffness continues to decrease gradually, ranging from a few percent for unidirectionally reinforced carbon composites to several tens of percents for multidirectional glass laminates. 3 7 Most onedimensional damage models for fibrereinforced composites only account for the effect of damage on the stiffness The degradation of the Poisson s ratio is not included in these models. Nevertheless this degradation has been observed and is not negligible. 17,18 Bandoh et al. showed that the Poisson s ratio of a carbon/epoxy UD laminate can drop by 50% under static tensile loading, 17 while Pidaparti and Vogt proved that the Poisson s ratio is a very sensitive parameter whilst monitoring fatigue damage in human bone. 18 In this paper, it is investigated whether or not the Poisson s ratio can be used as a sensitive indicator of (fatigue) Correspondence: W. Van Paepegem. damage in fibrereinforced composites for both static, cyclic and fatigue loading. Just like the stiffness, it can be measured accurately and nondestructively. Further, it gives information about the damage state of the offaxis plies in a multidirectional composite laminate. For longterm measurements, the use of strain gauges is less appropriate, but optical fibre sensor pads can be a viable alternative. In a first step, static tensile tests are performed on [0 /90 ] 2s glass/epoxy laminates, followed by cyclic loadingunloading tests and straincontrolled fatigue tests. MATERIAL AND TEST METHODS The material under study was a glass/epoxy composite. The glass reinforcement was a unidirectional Eglass fabric (Roviglas R17/475). In the fibre direction e 11, the reinforcement was 475 g/m 2, while in the direction e 22,the reinforcement was 17 g/m 2. The epoxy matrix was Araldite LY 556. Three stacking sequences were manufactured: [0 ] 8, [90 ] 8 and [0 /90 ] 2s with the angle referred to the direction e 11. The layups [0 ] 8 and [90 ] 8 were used for characterization in the orthotropic material directions, while [0 /90 ] 2s was used for the study of the Poisson s ratio. 269
2 270 W. VAN PAEPEGEM et al. All specimens were manufactured by vacuum assisted resin transfer moulding with a closed steel mould. The nominal thickness of all specimens was 3.0 mm and the fibre volume fraction was between 48 and 50%. The samples were cut to dimensions on a watercooled diamond tipped saw. The inplane elastic properties of the individual glass/epoxy lamina were determined by the dynamic modulus identification method described by Sol et al. 19,20 and are listed in Table 1. Apart from the dynamic modulus identification method, static tensile tests on the [0 ] 8 and [90 ] 8 layups have been performed to check the values of the elastic properties and to determine the static strengths. It is important to mention that the mechanical behaviour in the e 11 and e 22 direction is linear until failure. The tensile strength properties were determined from the [0 ] 8 and [90 ] 8 stacking sequence and are listed in Table 2. Based on this characterization of the individual glass/epoxy lamina, [0 /90 ] 2s crossply laminates were manufactured for investigation of the Poisson s ratio. STATIC MEASUREMENTS OF The elastic and strength properties of the [0 /90 ] 2s laminate were determined by quasistatic tensile tests on an Table 1 Inplane elastic properties of the individual glass/epoxy lamina E 11 (GPa) 38.9 E 22 (Gpa) 13.3 ν 12 [ ] G 12 (Gpa) 5.13 Table 2 Tensile strength properties of the individual glass/epoxy lamina X T (Mpa) ε11 ult [ ] Y T (Mpa) 36.5 ε22 ult [ ] Instron electromechanical testing machine. The tensile tests were displacementcontrolled with a displacement speed of 1 mm/min. The specimen geometry is illustrated in Fig. 1. The nominal specimen width was 34 mm and the thickness 3 mm. The gauge length was 140 mm. Two strain gauges were applied in the X and Y direction. The tests were done in accordance with ASTM D3039 Standard Test Method for Tensile Properties of Polymer Matrix Composite Materials. Figure 2 shows the stress strain curve for the [0 /90 ] 2s specimens IF4 and IF6. In the first measurement, the strain gauge signal was lost at about 1.0% longitudinal strain (due to debonding), but the load signal was measured until failure. The calculated failure stresses were and Mpa, respectively. The failure strain of specimen IF6 was (or 2.08%). The value of the elastic modulus was and GPa, respectively (determined by leastsquares linear fit for the strain range [0;0.0025]). The value measured by the dynamic modulus identification method was GPa for another specimen from the same batch of material. At a level of about 100 MPa axial stress, there is a small change in slope of the stress strain curve. The corresponding strain is slightly higher than (0.25%) which is the fracture strain of the 90 plies in the crossply laminate (see Table 2). The corresponding history of the Poisson s ratio versus is shown in Fig. 3. Although the axial stress strain curve is almost linear (Fig. 2), the Poisson s ratio is decreasing quite fast. This is due to early transverse matrix cracking of the 90 plies. Indeed the failure strain ε22 ult of the 90 plies equals only (see Table 2) and once the axial strain in these plies exceeds this threshold, the 90 plies are severely cracked. The estimated value of in the elastic regime is and 2 for IF4 and IF6, respectively. The calculated value of from the dynamic modulus identification method is The latter method is a mixed numerical/experimental method that aims to identify the engineering constants of orthotropic materials using measured resonant frequencies of freely suspended rectangular specimens. For the identification of the four orthotropic material constants, it is necessary 3 mm Y θ= 0 X Fig. 1 [0 /90 ] 2s glass/epoxy specimen s layout.
3 POISSON S RATIO AS AN INDICATOR OF DAMAGE 271 Stressstrain curve for static [0 /90 ] 2s tests IF4 and IF6 Forcedisplacement curve for cyclic [0 /90 ] 2s test IF3 500 IF4 IF6 = GPa σ xx [MPa] = GPa Force [kn] Fig. 2 Stress strain curve for the static tensile test of the [0 /90 ] 2s specimens IF4 and IF Displacement [mm] Fig. 4 Forcedisplacement curve for the [0 /90 ] 2s specimen IF3. Time history of and ε yy for cyclic [0 /90 ] 2s test IF versus for static [0 /90 ] 2s tests IF4 and IF6 static [0 /90 ] 2s test IF4 static [0 /90 ] 2s test IF ε yy and ε yy Fig. 3 Evolution of the Poisson s ratio in function of the longitudinal strain for the [0 /90 ] 2s specimens IF4 and IF6. to measure the first three resonant frequencies of a rectangular plate and the first resonant frequency of two beams, one cut along the longitudinal direction and the other cut along the transversal direction. Starting from an initial guess, the engineering constants are iteratively updated till a series of numerically computed resonance frequencies match the experimentally measured frequencies. This method is completely nondestructive which can explain the higher value for the Poisson s ratio. MEASUREMENTS OF UNDER CYCLIC LOADING In order to observe the behaviour of the Poisson s ratio under repeated loading, cyclic tensile tests are performed Time [s] Fig. 5 Time history of and ε yy for the [0 /90 ] 2s specimen IF3. The displacement speed is 2 mm/min and the load cycles between 1 kn and subsequent load levels of 20, 20, 25, 35, 35, 42, 45, 48 and 54.7 kn (failure load), as shown in Fig. 4. The small change of the slope in the curve at 10 kn corresponds with a longitudinal stress σ xx of MPa. This kneepoint could indeed be observed in the stress strain curves in Fig. 2. The corresponding time history of the measured longitudinal strain and the transverse strain ε yy for the cyclic tensile test on the [0 /90 ] 2s specimen IF3 is shown in Fig. 5. At the lowest loads of 1 kn, the transverses strain ε yy becomes slightly positive. This is not caused by improper calibration of the strain gauges. The strain measurement channels are calibrated for each strain gauge with a precision shunt resistance. It will be shown in subsequent figures that this effect is very reproducible. Both the failure stress and failure strain are higher than in the quasistatic tensile tests. The failure stress here is
4 272 W. VAN PAEPEGEM et al. Time history of and for cyclic [0 /90 ] 2s test IF3, Time [s] Fig. 6 Time history of the Poisson s ratio for the [0 /90 ] 2s specimen IF3. Fig. 8 Instrumentation of the [0 /90 ] 2s glass/epoxy specimens. versus for cyclic [0 /90 ] 2s test IF3 cyclic [0 /90 ] 2s test IF3 static [0 /90 ] 2s test IF4 static [0 /90 ] 2s test IF6 value must be stress dependent because no further damage occurs during unloading. νxy Fig. 7 Evolution of the Poisson s ratio in function of the longitudinal strain for the cyclic [0 /90 ] 2s test IF MPa and the failure strain (or 2.93%). This strengthening effect might be due to better fibre alignment. A similar phenomenon was already reported by the authors for cyclic loading/unloading tests of [+45/ 45] 2s glass/epoxy laminates. 21,22 Figure 6 shows the corresponding time history of the Poisson s ratio. In the region of low forces (and thus low strains ), the Poisson s ratio becomes negative, due to the slightly positive value of the transverse strain ε yy for small loading values (see Fig. 5). In Fig. 7, the evolution of the Poisson s ratio is plotted against the longitudinal strain, together with its evolution in the quasistatic tensile tests IF4 and IF6 (see Fig. 3). It can be clearly seen that the maxima of the cyclic curves follow the static curve very well. As the Poisson s ratio changes drastically during unloading, its MEASUREMENTS OF UNDER FATIGUE LOADING In order to assess the sensitivity of the Poisson s ratio for fatigue damage, tension tension fatigue tests have been conducted on the same material. The specimen geometry was the same as shown in Fig. 1, but the longitudinal strain gauge has been replaced by an extensometer. The fatigue tests were straincontrolled, so that the measurement of the transverse strain ε yy immediately yields the value of the Poisson s ratio. The maximum strain level was chosen (0.6%), because this strain level is slightly higher than the kneepoint in the static stress strain curve (see Fig. 2). Using a strain ratio R of 0.1 (similar to the stress ratio in fatigue), the minimum strain level is (0.06%). The fatigue tests were done at 2 Hz on an Instron servohydraulic testing machine. Figure 8 shows the clamped specimen with its instrumentation. The extensometer measures the longitudinal strain, the transverse strain gauge measures the transverse strain and a thermocouple monitors the surface temperature of the composite laminate. Load and displacement were measured by the servohydraulic machine control. Normally, the life time of strain gauges in fatigue is very limited, because the limit strain levels they can endure in fatigue, are very much reduced compared to static operation. However, in this case the transverse strain levels were very small (a few hundred microstrains) and no temperature rise of the surface was detected from the thermocouple.
5 POISSON S RATIO AS AN INDICATOR OF DAMAGE 273 Stressstrain curve for [0 /90 ] 2s fatigue test W_090_7 versus for [0 /90 ] 2s fatigue test W_090_ = GPa static [0 /90 ] 2s test IF4 static [0 /90 ] 2s test IF6 [0 /90 ] 2s fatigue test W_090_7: cycle [0 /90 ] 2s fatigue test W_090_7: cycle [0 /90 ] 2s fatigue test W_090_7: cycle σ xx [MPa] = GPa static [0 /90 ] 2s test W_090_7: cycle 0 intermediate static [0 /90 ] 2s test W_090_7: cycle Fig. 9 Stress strain curve for the initial and intermediate static tensile tests of the [0 /90 ] 2s fatigue test W Fig. 11 Evolution of the Poisson s ratio in function of the longitudinal strain for the 0 /90 ] 2s specimen W at three chosen intervals in the fatigue test versus time for [0 /90 ] 2s fatigue test W_090_7 [0 /90 ] 2s fatigue test W_090_7: cycle [0 /90 ] 2s fatigue test W_090_7: cycle [0 /90 ] 2s fatigue test W_090_7: cycle Time Fig. 10 Time history of the Poisson s ratio for the [0 /90 ] 2s specimen W at three chosen intervals in the fatigue test. The signals of load, displacement, extensometer, strain gauge and temperature were each sampled at 100 Hz every 5 min for five subsequent loading cycles with a National Instruments NI DAQPAD 6052E measurement card and LabVIEW software. For the first fatigue test W 090 7, 7500 loading cycles were applied. The stress strain curve was measured before fatigue testing, but only to a very low axial strain of (0.1%), because the failure strain of the 90 plies is only (0.25%) (see Table 2). After stopping the fatigue test, the same static tensile test was repeated. Figure 9 shows the measured static stress strain curves for cycle 0 and cycle A degradation of the axial stiffness is observed from to GPa. Figure 10 shows the time history of the Poisson s ratio at three chosen intervals in the fatigue test. The ab scissa shows the sample number of the data acquisition (proportional with time). Five full cycles correspond with 2.5 s (2 Hz). The behaviour is very similar with that in cyclic loadingunloading tests (see Fig. 6). The maximum value of the Poisson s ratio is clearly decreasing with increasing loading cycles, while the negative peaks are increasing as well. In Fig. 11, the evolution of the Poisson s ratio is again plotted against the longitudinal strain for the same sets of five cycles as shown in Fig. 10. The shape of the loadingunloading curves is very similar to the one showed in Fig. 7. It must be noticed as well that the Poisson s ratio shows a sharp decline during the first loading cycles. After only 600 cycles, the value has already decreased considerably. To be sure that the shape of the curves is not due to strain rate effects, the evolution of the Poisson s ratio is plotted against the longitudinal strain for the static tensile tests that were done before the fatigue testing and after 7500 cycles. Figure 12 shows that the initial Poisson s ratio is about 0.16 [ ], while after 7500 cycles, the shape of the curve appears again. It is important to stress the fact that the maximum applied strain during these static tensile tests was only (0.1%), in order to be sure that no damage was introduced into the specimen before fatigue testing. Indeed, this strain level is wel below the transverse failure strain of the 90 plies (0.0025, see Table 2). For the second fatigue test W 090 8, loading cycles were applied. The stress strain curve was measured before fatigue testing, but again only up till a very low axial strain of (0.1%). At two intermediate loading cycles, the fatigue test was stopped and the same static tensile test was repeated.
6 274 W. VAN PAEPEGEM et al. versus for [0 /90 ] 2s fatigue test W_090_7 versus time for [0 /90 ] 2s fatigue test W_090_8 [0 /90 ] 2s fatigue test W_090_8: cycle [0 /90 ] 2s fatigue test W_090_8: cycle [0 /90 ] 2s fatigue test W_090_8: cycle static [0 /90 ] 2s test W_090_7: cycle 0 intermediate static [0 /90 ] 2s test W_090_7: cycle Fig. 12 Evolution of the Poisson s ratio in function of the longitudinal strain for the initial and intermediate static tensile tests of the [0 /90 ] 2s fatigue test W Time Fig. 14 Time history of the Poisson s ratio for the [0 /90 ] 2s specimen W at three chosen intervals in the fatigue test. σ xx [MPa] Stressstrain curve for [0 /90 ] 2s fatigue test W_090_8 static [0 /90 ] 2s test W_090_8: cycle 0 intermediate static [0 /90 ] 2s test W_090_8: cycle 7500 intermediate static [0 /90 ] 2s test W_090_8: cycle = GPa = GPa = GPa Fig. 13 Stress strain curve for the initial and intermediate static tensile tests of the [0 /90 ] 2s fatigue test W versus for [0 /90 ] 2s fatigue test W_090_8 static [0 /90 ] 2s test IF4 static [0 /90 ] 2s test IF6 [0 /90 ] 2s fatigue test W_090_8: cycle [0 /90 ] 2s fatigue test W_090_8: cycle [0 /90 ] 2s fatigue test W_090_8: cycle Fig. 15 Evolution of the Poisson s ratio in function of the longitudinal strain for the 0 /90 ] 2s specimen W at three chosen intervals in the fatigue test. Figure 13 shows the stress strain curves before fatigue testing, and at cycle 7500 and cycle The initial stiffness of GPa decreases to GPa, and further to GPa. The comparison of the stiffness degradations in Fig. 13 and Fig. 9 is not straightforward due to the very different strain scale. In Fig. 13 a leastsquares linear fit to the full strain range [ ] has been done. If only the strain interval [ ] is used for determination of the Young s modulus, the values are and GPa, respectively. Figure 14 shows the time history of the Poisson s ratio for three chosen intervals in the fatigue test. The abscis shows again the sample number of the data acquisition, but the five plotted cycles correspond again with 2.5 s (2 Hz). The behaviour is very similar with that in cyclic loadingunloading tests (see Fig. 7). In Fig. 15, the evolution of the Poisson s ratio is again plotted against the longitudinal strain for the same sets of five cycles as shown in Fig. 14. The correspondence with Fig. 11 is again very good. It seems that both the maximum and minimum value of the Poisson s ratio are affected by the fatigue damage and could be a usable damage variable. Here again, the evolution of the Poisson s ratio versus longitudinal strain was measured under static loading conditions as well, to eliminate strain rate effects. However, the intermediate static tests were now performed up to a maximum strain of (0.6%), as opposed to Fig. 12. Figure 16 shows that the initial Poisson s ratio is now about [ ]. The scatter is quite large in the initial strain regime, due to the very low axial strains and even lower transverse strains ε yy. However, at an axial strain of
7 P O I S S O N S R AT I O A S A N I N D I C ATO R O F DA M AG E 0.001, the Poisson s ratio converges to a more or less constant value. In the intermediate static tests at cycles 7500 and , the same strain range [ ] as in the fatigue loading cycles has been applied. The same shape of the curve appears. More fatigue tests have been done that confirm the behaviour discussed above. Finally, some tests were taken up till final failure. The glass/epoxy composite is fully cracked then and turns white. After cycles failure occurs by fracture of the fibres. The typical damage patterns are shown in Fig. 17 for cycles (left) and at failure ( cycles). In this stage of severe damage, the evolution of the Poisson s ratio versus longitudinal strain still shows the same shape, but the amplitude is about 10 times smaller, as shown in Fig. 18. Some precaution is also necessary in this case. Due to the damaged surface, the bonding quality of the transverse strain gauge will have deteriorated, so that the strain transfer from the composite surface to the strain gauge is not reliable anymore. Perhaps a biaxial extensometer could be used to solve this problem. However, as the same shape still appears, it can be assumed that the measurements are still valid. CONCLUSIONS It has been demonstrated that both the amplitude and shape of the curve change when damage is present in a composite laminate. The static evolution of the Poisson s ratio is the envelope that encloses the cyclic curves. Also, the degradation of the Poisson s ratio is much larger than that of the stiffness. Further research is required to investigate the value of using the Poisson s ratio as a damage indicator for other material combinations than glass/epoxy. νxy versus εxx for [0 /90 ]2s fatigue test W_090_ εxx  intermediate static [0 /90 ]2s test W_090_4: cycle intermediate static [0 /90 ]2s test W_090_4: cycle νxy νxy νxy versus εxx for [0 /90 ]2s fatigue test W_0_90_ static [0 /90 ]2s test W_090_8: cycle 0 intermediate static [0 /90 ]2s test W_090_8: cycle 7500 intermediate static [0 /90 ]2s test W_090_8: cycle εxx Fig. 18 Evolution of the Poisson s ratio in function of the longitudinal strain εxx for the intermediate static tensile tests of the [0 /90 ]2s fatigue test W Fig. 17 Typical damage patterns in the [0 /90 ]2s specimens (a) close to failure, and (b) after failure. c 2007 Blackwell Publishing Ltd. Fatigue Fract Engng Mater Struct 30, Fig. 16 Evolution of the Poisson s ratio in function of the longitudinal strain for the initial and intermediate static tensile tests of the [0 /90 ]2s fatigue test W
8 276 W. VAN PAEPEGEM et al. Acknowledgements The author W. V. P. gratefully acknowledges his finance through a grant of the Fund for Scientific Research Flanders (F.W.O.) Procedings on CDROM. The authors also express their gratitude to Syncoglas for their support and technical collaboration. REFERENCES 1 Mallick, P. K. (1997) Composites Engineering Handbook. Marcel Dekker Inc., New York. 2 Herakovich, C. T. (1998) Mechanics of Fibrous Composites. John Wiley & Sons, Inc., New York. 3 Schulte, K., Baron, Ch., Neubert, H., et al (1985) Damage development in carbon fibre epoxy laminates : Cyclic loading. In : Proceedings of the MRSsymposium Advanced Materials for Transport, November 1985, Strassbourg, pp Schulte, K., Reese, E. and Chou, T.W. (1987) Fatigue behaviour and damage development in woven fabric and hybrid fabric composites. In : Sixth International Conference on Composite Materials (ICCMVI) & Second European Conference on Composite Materials (ECCMII) (Edited by F. L. Matthews, N. C. R. Buskell, J. M. Hodgkinson, and J. Morton) Vol. 4. Proceedings, July 1987, Elsevier, London, UK, pp Schulte, K. (1984) Stiffness reduction and development of longitudinal cracks during fatigue loading of composite laminates. In : Mechanical characterisation of load bearing fibre composite laminates. Proceedings of the European Mechanics Colloquium 182, August 1984, Brussels, (Edited by A. H. Cardon and G. Verchery) Elsevier, Belgium, pp Fujii, T., Amijima, S. and Okubo, K. (1993) Microscopic fatigue processes in a plainweave glassfibre composite. Comp. Sci. Technol. 49, Pandita, S. D., Huysmans, G., Wevers, M. and Verpoest, I. (2000) Tensile fatigue behaviour of glassplain weave fabric composites in the on and offaxis directions. Proceedings of the Fifth International Conference on Textile Composites, Leuven, Belgium, September Sidoroff, F. and Subagio, B. (1987) Fatigue damage modelling of composite materials from bending tests. In : Sixth International Conference on Composite Materials (ICCMVI) & Second European Conference on Composite Materials (ECCMII) (Edited by F. L. Matthews, N. C. R. Buskell, J. M. Hodgkinson, and J. Morton) Vol. 4. Proceedings, July 1987, Elsevier, London, UK, pp Vieillevigne, S., Jeulin, D., Renard, J. and Sicot, N. (1997) Modelling of the fatigue behaviour of a unidirectional glass epoxy composite submitted to fatigue loadings. In: International Conference on fatigue of composites (Edited by S. Degallaix, C. Bathias and R. Fougères). Proceedings, 35 June 1997, La Société Française de Métallurgie et de Matériaux, Paris, France, pp Kawai, M. (1999) Damage mechanics model for offaxis fatigue behavior of unidirectional carbon fiberreinforced composites at room and high temperatures. In: Proceedings of the Twelfth International Conference on Composite Materials (ICCM12) (Edited by T. Massard and A. Vautrin). Paris, France, 5 9 July 1999, pp Hwang, W. and Han, K. S. (1986) Fatigue of composites  Fatigue modulus concept and life prediction. J. Comp. Mater. 20, Hwang, W. and Han, K. S. (1986) Cumulative damage models and multistress fatigue life prediction. J. Comp. Mater. 20, Whitworth, H. A. (1987) Modelling stiffness reduction of graphite epoxy composite laminates. J. Comp. Mater. 21, Yang, J. N., Jones, D. L., Yang, S. H. and Meskini, A. (1990) A stiffness degradation model for graphite/epoxy laminates. J. Comp. Mater. 24, Brøndsted, P., Andersen, S. I. and Lilholt, H. (1997) Fatigue damage accumulation and lifetime prediction of GFRP materials under block loading and stochastic loading. In : Polymeric Composites  Expanding the Limits. Proceedings of the 18th Risø International Symposium on Materials Science, 15 September 1997 (Edited by S. I. Andersen, P. Brøndsted, H. Lilholt, Aa. Lystrup, J. T. Rheinländer, B. F. Sørensen and H. Toftegaard). Risø International Laboratory, Roskilde, Denmark, pp Brondsted, P., Lilholt, H. and Andersen, S. I. (1997) Fatigue damage prediction by measurements of the stiffness degradation in polymer matrix composites. In : International Conference on fatigue of composites (Edited by S. Degallaix, C. Bathias and R. Fougères) Proceedings, 3 5 June 1997, La Société Française de Métallurgie et de Matériaux, Paris, France, pp Bandoh, S., Matsumura, K., Zako, M., Shiino, T. and Kurashiki, T. (2001) On the detection of fatigue damage in CFRP by measuring Poisson s ratio. In: Eighth International Conference on Composites Engineering (ICCE/8) (Edited by D. Hui) Proceedings. Tenerife, Spain, 5 11 August 2001, pp Pidaparti, R. M. and Vogt, A. (2002) Experimental investigation of Poisson s ratio as a damage parameter for bone fatigue. J. Biomed. Mater. Res. Part A 59, Sol, H. and de Wilde, W. P. (1988) Identification of elastic properties of composite materials using resonant frequencies. In : Proceedings of the International Conference Computer Aided Design in Composite Material Technology (Edited by C.A. Brebbia, W. P. de Wilde and W. R. Blain) 1988, SpringerVerlag, Southampton, pp Sol, H. (1990) Identification of the complex moduli of composite materials by a mixed numerical/experimental method. In : Proceedings of the second International Conference on Computer Aided Design in Composite Material Technology (Edited by W. P. de Wilde and W. R. Blain) April 1990, SpringerVerlag, Brussels, pp Van Paepegem, W., De Baere, I. and Degrieck, J. (2005) Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part I: Experimental results. Comp. Sci. Technol. 66, Van Paepegem, W., De Baere, I. and Degrieck, J. (2005) Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations. Comp. Sci. Technol. 66,
Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationNonlinear correction to the bending stiffness of a damaged composite beam
Van Paepegem, W., Decaene, R. and Degrieck, J. (5). Nonlinear correction to te bending stiffness of a damaged composite beam. Nonlinear correction to te bending stiffness of a damaged composite beam W.
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationInsitu local strain measurement in textile composites with embedded optical fibre sensors
Insitu local strain measurement in textile composites with embedded optical fibre sensors S. Daggumati, E. Voet, I. De Baere, W. Van Paepegem & J. Degrieck Ghent University, Department of Materials Science
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationNUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION
NUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION Fabrice PIERRON*, François CERISIER*, and Michel GRÉDIAC** * SMS/ Département Mécanique et Matériaux, École Nationale Supérieure
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationA SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST
A SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST P. Robinson The Composites Centre, Department of Aeronautics, Imperial College London South Kensington, London, SW7 2AZ, UK p.robinson@imperial.ac.uk
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationSPECTRUM FATIGUE LIFETIME AND RESIDUAL STRENGTH FOR FIBERGLASS LAMINATES IN TENSION
AIAA225 SPECTRUM FATIGUE LIFETIME AND RESIDUAL STRENGTH FOR FIBERGLASS LAMINATES IN TENSION Neil Wahl Montana Tech of The University of Montana Butte, Montana 597 Daniel Samborsky John Mandell Douglas
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationAgnieszka Bondyra, Pawe Gotowicki
Journal of KONES Powertrain and Transport, Vol. 17, No. 1 21 INFLUENCE OF A CROSSHEAD RATE AND A NUMBER OF STRESS CYCLES ON MEASUREMENT RESULTS IN THE INPLANE SHEAR TEST FOR A CROSSPLY VINYLESTERCARBON
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationSUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES
SUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES T.R. Emery 1, J. M. DulieuBarton 1, P.R. Cunningham 2 1 University of Southampton, School of Engineering Sciences, SO17 1BJ, UK
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationStatic and Time Dependent Failure of Fibre Reinforced Elastomeric Components. Salim Mirza Element Materials Technology Hitchin, UK
Static and Time Dependent Failure of Fibre Reinforced Elastomeric Components Salim Mirza Element Materials Technology Hitchin, UK Introduction Fibre reinforced elastomers are used in many applications,
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationThe Power of Ultrasonic Characterisation for Completely Assessing the Elastic Properties of Materials
11th European Conference on NonDestructive Testing (ECNDT 214), October 61, 214, Prague, Czech Republic The Power of Ultrasonic Characterisation for Completely Assessing the Elastic Properties of Materials
More informationInterlaminar fracture characterization in composite materials by using acoustic emission
5th International Symposium on NDT in Aerospace, 1315th November 2013, Singapore Interlaminar fracture characterization in composite materials by using acoustic emission Ian SILVERSIDES 1, Ahmed MASLOUHI
More informationIntroduction to scaling issues of damage and fracture in wind turbine blades
Introduction to scaling issues of damage and fracture in wind turbine blades Bent F. Sørensen Composites and Materials Mechanics Section Department of Wind Energy Technical University of Denmark Risø Campus,
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationEXPERIMENTAL AND NUMERICAL STUDY OF THE ENERGY ABSORPTION CAPACITY OF PULTRUDED COMPOSITE TUBES
EXPERIMENTAL AND NUMERICAL STUDY OF THE ENERGY ABSORPTION CAPACITY OF PULTRUDED COMPOSITE TUBES D. Kakogiannis 1, D. Van Hemelrijck 1, J. Wastiels 1, S. Palanivelu 2, W. Van Paepegem 2, K. De Wolf 3, J.
More informationFracture Mechanics Analysis of Composite Microcracking: Experimental Results in Fatigue
Proceedings of the 5 th Technical Conference on Composite Materials, American Society of Composites, East Lansing, Michigan, June 1114, 1990). Fracture Mechanics Analysis of Composite Microcracking: Experimental
More informationSHEAR CAPACITY OF REINFORCED CONCRETE COLUMNS RETROFITTED WITH VERY FLEXIBLE FIBER REINFORCED POLYMER WITH VERY LOW YOUNG S MODULUS
SHEAR CAPACITY OF REINFORCED CONCRETE COLUMNS RETROFITTED WITH VERY FLEXILE FIER REINFORCED POLYMER WITH VERY LOW YOUNG S MODULUS Hu Shaoqing Supervisor: Susumu KONO ** MEE8165 ASTRACT FRP with low Young
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationIMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS OBTAINED WITH LMS SAMTECH SAMCEF
V ECCOMAS Thematic Conference on the Mechanical Response of Composites COMPOSITES 015 S.R. Hallett and J.J.C. Remmers (Editors) IMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationAE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF HOOP STRESSES FOR A THINWALL PRESSURE VESSEL
Objective AE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF OOP STRESSES FOR A TINWA PRESSURE VESSE This experiment will allow you to investigate hoop and axial stress/strain relations
More informationID1160 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING
ID116 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING K. Minnaar and M. Zhou = School of Mechanical Engineering Georgia Institute
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationUSING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE
Volume II: Fatigue, Fracture and Ceramic Matrix Composites USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE A. D. Resnyansky and
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationDIGITAL IMAGE CORRELATION TECHNIQUE IN MEASURING DEFORMATION AND FAILURE OF COMPOSITE AND ADHESIVE
DIGITAL IMAGE CORRELATION TECHNIQUE IN MEASURING DEFORMATION AND FAILURE OF COMPOSITE AND ADHESIVE Ab Ghani A. F Sustainable Maintenance Engineering Research Group, Universiti Teknikal Malaysia Melaka,
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More information1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine Spring 2004 LABORATORY ASSIGNMENT NUMBER 6
1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine MIT Spring 2004 LABORATORY ASSIGNMENT NUMBER 6 COMPRESSION TESTING AND ANISOTROPY OF WOOD Purpose: Reading: During this laboratory
More informationFrequency Response of Composite Laminates at Various Boundary Conditions
International Journal of Engineering Science Invention (IJESI) ISSN (Online): 2319 6734, ISSN (Print): 2319 6726 www.ijesi.org ǁ PP.1115 Frequency Response of Composite Laminates at Various Boundary Conditions
More informationDRAPING SIMULATION. Recent achievements and future trends. Dr. Sylvain Bel LGCIE University Lyon 1
DRAPING SIMULATION Recent achievements and future trends 1 Dr. Sylvain Bel LGCIE University Lyon 1 2 DRAPING SIMULATION Why? How? What? DRAPING SIMULATION WHY? Clamps Punch Fabric Die 1 2 Resin 3 4 Fig.
More informationEnergy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing the effect of residual stresses
International Journal of Adhesion & Adhesives 20 (1999) 59 70 International Journal of Adhesion & Adhesives Energy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing
More informationValidation of the Resonalyser method: an inverse method for material identification
Validation of the Resonalyser method: an inverse method for material identification T. Lauwagie, H. Sol,. Roebben 3, W. Heylen and Y. Shi Katholieke Universiteit Leuven (KUL) Department of Mechanical ngineering
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationCHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS
Oral Reference Number: ICF100942OR CHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS T. Kevin O Brien U.S. Army Research Laboratory Vehicle Technology Directorate
More informationS. Srinivasan, Technip Offshore, Inc., Houston, TX
9 th ASCE Specialty Conerence on Probabilistic Mechanics and Structural Reliability PROBABILISTIC FAILURE PREDICTION OF FILAMENTWOUND GLASSFIBER Abstract REINFORCED COMPOSITE TUBES UNDER BIAXIAL LOADING
More informationLAMB WAVE RESPONSE OF FATIGUED COMPOSITE SAMPLES. Reveiw of Progress in Quantitative Nondestructive Evaluation, Vol 13B (1994) pp.
LAMB WAVE RESPONSE OF FATIGUED COMPOSITE SAMPLES Reveiw of Progress in Quantitative Nondestructive Evaluation, Vol 13B (1994) pp. 12611266 INTRODUCTION Michael D. Seale and Barry T. Smith Departments
More informationA Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber
A Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber Kibong Han Mechatronics Department, Jungwon University, 85 Munmuro, Goesangun, South Korea.
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationTensile Stress Acoustic Constants of Unidirectional Graphite/Epoxy Composites
Tensile Stress Acoustic Constants of Unidirectional Graphite/Epoxy Composites Journal of Reinforced Plastics and Composites, Vol. 9 (March, 1990) pp. 127133 W. H. PROSSER NASA Langley Research Center
More informationA New Methodology for Fiber Optic Strain Gage Measurements and its Characterization ABSTRACT
.3 A New Methodology for Fiber Optic Strain Gage Measurements and its Characterization Van Roosbroeck Jan, C. Chojetzki, J. Vlekken, E. Voet, M. Voet Fiber Optic Sensors and Sensing Systems (FOS&S), Cipalstraat
More informationA STUDY ON FATIGUE CRACK GROWTH IN CONCRETE IN THE PREPARIS REGION
VIII International Conference on Fracture Mechanics of Concrete and Concrete Structures FraMCoS8 J.G.M. Van Mier, G. Ruiz, C. Andrade, R.C. Yu and X.X. Zhang (Eds) A STUDY ON FATIGUE CRACK GROWTH IN CONCRETE
More informationElastic parameters prediction under dynamic loading based on the. unit cell of composites considering end constraint effect
Elastic parameters prediction under dynamic loading based on the unit cell of composites considering end constraint effect Wang Meng 1,, Fei Qingguo 1,, Zhang Peiwei 1, (1. Institute of Aerospace Machinery
More informationA FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
TRENDS IN COMPUTATIONAL STRUCTURAL MECHANICS W.A. Wall, K.U. Bletzinger and K. Schweizerhof (Eds.) c CIMNE, Barcelona, Spain 2001 A FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
More informationPullout Tests of Geogrids Embedded in Noncohesive Soil
Archives of HydroEngineering and Environmental Mechanics Vol. 51 (2004), No. 2, pp. 135 147 Pullout Tests of Geogrids Embedded in Noncohesive Soil Angelika Duszyńska, Adam F. Bolt Gdansk University of
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationThe Relationship between the Applied Torque and Stresses in PostTension Structures
ECNDT 6  Poster 218 The Relationship between the Applied Torque and Stresses in PostTension Structures Fui Kiew LIEW, Sinin HAMDAN * and Mohd. Shahril OSMAN, Faculty of Engineering, Universiti Malaysia
More informationMULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS
MULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS F.X. Irisarri, J.F. Maire* and N. Carrere ONERA, 9 av. de la Division Leclerc, 930 Châtillon, France francoisxavier.irisarri@onera.fr,
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More informationAPPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN
28 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES APPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN Tuyen Tran*, Dan Simkins**, Shen Hin Lim*,
More informationMonitoring Fatigue Damage in CFRP Using Ultrasonic Birefringence
19 th World Conference on NonDestructive Testing 2016 Monitoring Fatigue Damage in CFRP Using Ultrasonic Birefringence Peter FEY 1, Marc KREUTZBRUCK 1 1 Universität Stuttgart, Stuttgart, Germany Contact
More informationADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF COMPOSITES
NAFEMS WORLD CONGRESS 13, SALZBURG, AUSTRIA ADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF M. Bruyneel, J.P. Delsemme, P. Jetteur (LMS Samtech, Belgium); A.C. Goupil (ISMANS, France). Dr. Ir. M. Bruyneel,
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationMalaysia Phone: ; Fax:
International Conference on Mechanical Engineering Research (ICMER013), 13 July 013 Bukit Gambang Resort City, Kuantan, Pahang, Malaysia Organized By Faculty of Mechanical Engineering, Universiti Malaysia
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationPrediction of Compressive Strength of Fibrous Composites Using Two Different Approaches
Jordan Journal of Civil Engineering, Volume 8, No. 2, 214 Prediction of Compressive Strength of Fibrous Composites Using Two Different Approaches Yousef S. Al Rjoub 1) * and Karim S. Numayr 2) 1) Civil
More informationUniversity of Southampton Research Repository eprints Soton
University of Southampton Research Repository eprints Soton Copyright and Moral Rights for this thesis are retained by the author and/or other copyright owners. A copy can be downloaded for personal noncommercial
More informationPLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS PLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES P. Tesinova Technical University of Liberec, Faculty of Textile
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationEXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS
EXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS Kevin L. Peil +, Ever J. Barbero +, Eduardo M. Sosa* + Department of Mechanical and Aerospace Engineering, West Virginia University (WVU), Morgantown,
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationFinite ElementBased Failure Models for Carbon/Epoxy Tape Composites
Finite ElementBased Failure Models for Carbon/Epoxy Tape Composites A Master Thesis Presented to The Academic Faculty by Guillaume Seon In Partial Fulfillment of the Requirements for the Degree Master
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationThis is a publisherdeposited version published in: Eprints ID: 4094
This is a publisherdeposited version published in: http://oatao.univtoulouse.fr/ Eprints ID: 4094 To cite this document: WEISS Ambrosius, TRABELSI Walid, MICHEL Laurent, BARRAU JeanJacques, MAHDI Stéphane.
More informationA PROTOCOL FOR DETERMINATION OF THE ADHESIVE FRACTURE TOUGHNESS OF FLEXIBLE LAMINATES BY PEEL TESTING: FIXED ARM AND TPEEL METHODS
1 A PROTOCOL FOR DETERMINATION OF THE ADHESIVE FRACTURE TOUGHNESS OF FLEXIBLE LAMINATES BY PEEL TESTING: FIXED ARM AND TPEEL METHODS An ESIS Protocol Revised June 2007, Nov 2010 D R Moore, J G Williams
More informationSpecial edition paper
Development of New Aseismatic Structure Using Escalators Kazunori Sasaki* Atsushi Hayashi* Hajime Yoshida** Toru Masuda* Aseismatic reinforcement work is often carried out in parallel with improvement
More information